#------------------------------------------------------------------------------
#$Date: 2016-03-23 20:38:18 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179416 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/13/4331333.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4331333
loop_
_publ_author_name
'Ming-Yan Chung'
'Chi-Shen Lee'
_publ_contact_author_address
;Department of Applied Chemistry, National Chiao Tung University, 
1001 University Rd., Hsinchu 30010, Taiwan.
;
_publ_contact_author_email       chishen@mail.nctu.edu.tw
_publ_contact_author_fax         886-3-5723764
_publ_contact_author_name        'Chi-Shen Lee'
_publ_contact_author_phone       886-3-5712121
_publ_section_title
;
 Multinary Selenides with Unusual Coordination Environment of Bismuth
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              13328
_journal_page_last               13333
_journal_paper_doi               10.1021/ic302027b
_journal_volume                  51
_journal_year                    2012
_chemical_formula_sum            'Bi7 Ge2 Se24 Sr8 Y'
_chemical_formula_weight         4292.95
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           33
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'P 2c -2n'
_symmetry_space_group_name_H-M   'P n a 21'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   12.8349(15)
_cell_length_b                   29.068(3)
_cell_length_c                   12.8475(15)
_cell_measurement_temperature    273(2)
_cell_volume                     4793.2(9)
_computing_cell_refinement       'SAINT V7.60A (Bruker AXS)'
_computing_data_collection       APEX2
_computing_data_reduction        'SAINT V7.60A (Bruker AXS)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      273(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  CCD
_diffrn_measurement_method       'profile data from θ/2θ scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0941
_diffrn_reflns_av_sigmaI/netI    0.0735
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       34
_diffrn_reflns_limit_k_min       -33
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            41421
_diffrn_reflns_theta_full        25.08
_diffrn_reflns_theta_max         25.08
_diffrn_reflns_theta_min         1.40
_exptl_absorpt_coefficient_mu    55.069
_exptl_absorpt_correction_T_max  0.110
_exptl_absorpt_correction_T_min  0.082
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    5.949
_exptl_crystal_description       rod
_exptl_crystal_F_000             7216
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.04
_refine_diff_density_max         4.905
_refine_diff_density_min         -3.792
_refine_diff_density_rms         0.462
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.35(6)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.041
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     381
_refine_ls_number_reflns         8487
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.041
_refine_ls_R_factor_all          0.1150
_refine_ls_R_factor_gt           0.0499
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0377P)²+80.5513P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1010
_refine_ls_wR_factor_ref         0.1256
_reflns_number_gt                4576
_reflns_number_total             8487
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic302027b_si_002_3.cif
_cod_data_source_block           srygebise
_cod_original_cell_volume        4793.3(10)
_cod_database_code               4331333
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Sr1A Sr 0.5188(2) -0.08513(10) -0.2738(8) 0.0222(6) Uani 0.90 1 d P
Y1A Y 0.5188(2) -0.08513(10) -0.2738(8) 0.0222(6) Uani 0.11 1 d P
Sr1B Sr 0.4737(6) 0.0930(3) -0.4410(6) 0.0149(16) Uani 0.90 1 d P
Y1B Y 0.4737(6) 0.0930(3) -0.4410(6) 0.0149(16) Uani 0.11 1 d P
Sr1C Sr 0.5218(7) -0.0903(3) -0.6067(7) 0.035(2) Uani 0.90 1 d P
Y1C Y 0.5218(7) -0.0903(3) -0.6067(7) 0.035(2) Uani 0.11 1 d P
Sr2A Sr 0.81448(18) 0.15284(8) 0.2266(9) 0.0172(6) Uani 0.90 1 d P
Y2A Y 0.81448(18) 0.15284(8) 0.2266(9) 0.0172(6) Uani 0.11 1 d P
Sr2B Sr 0.8093(7) 0.1553(3) -0.4407(6) 0.020(2) Uani 0.90 1 d P
Y2B Y 0.8093(7) 0.1553(3) -0.4407(6) 0.020(2) Uani 0.11 1 d P
Sr2C Sr 0.8081(7) 0.1560(3) -0.1052(7) 0.0174(19) Uani 0.90 1 d P
Y2C Y 0.8081(7) 0.1560(3) -0.1052(7) 0.0174(19) Uani 0.11 1 d P
Sr3A Sr 0.17251(18) 0.18341(9) 0.2257(9) 0.0172(6) Uani 0.90 1 d P
Y3A Y 0.17251(18) 0.18341(9) 0.2257(9) 0.0172(6) Uani 0.11 1 d P
Sr3B Sr 0.1762(7) 0.1868(3) -0.4425(6) 0.0150(19) Uani 0.90 1 d P
Y3B Y 0.1762(7) 0.1868(3) -0.4425(6) 0.0150(19) Uani 0.11 1 d P
Sr3C Sr 0.1770(7) 0.1868(3) -0.1035(7) 0.0165(19) Uani 0.90 1 d P
Y3C Y 0.1770(7) 0.1868(3) -0.1035(7) 0.0165(19) Uani 0.11 1 d P
Ge4A Ge 0.9262(7) 0.2845(3) 0.0739(6) 0.015(2) Uani 1 1 d .
Bi4B Bi 0.94511(8) 0.27368(3) -0.2723(4) 0.0196(2) Uani 1 1 d .
Ge4C Ge 0.9265(7) 0.2845(3) 0.3820(6) 0.0150(19) Uani 1 1 d .
Bi5A Bi 0.05386(8) 0.06739(3) -0.2736(4) 0.0171(2) Uani 1 1 d .
Bi5B Bi 0.0541(3) 0.06480(12) 0.0582(2) 0.0172(8) Uani 1 1 d .
Bi5C Bi 0.0539(3) 0.06479(12) -0.6050(2) 0.0177(8) Uani 1 1 d .
Bi6A Bi 0.73198(8) 0.02685(4) -0.2740(4) 0.0263(3) Uani 1 1 d .
Bi6B Bi 0.2657(3) -0.02424(13) -0.4379(3) 0.0225(9) Uani 1 1 d .
Bi6C Bi 0.7343(3) 0.02410(12) -0.6094(3) 0.0210(8) Uani 1 1 d .
Se1A Se 0.6485(2) 0.11475(9) -0.2749(9) 0.0189(7) Uani 1 1 d .
Se1B Se 0.3474(7) -0.1120(3) -0.4379(6) 0.016(2) Uani 1 1 d .
Se1C Se 0.6522(7) 0.1119(3) -0.6099(7) 0.017(2) Uani 1 1 d .
Se2A Se 0.0019(2) 0.16022(9) -0.2752(8) 0.0148(6) Uani 1 1 d .
Se2B Se 0.0032(8) 0.1558(3) 0.0601(6) 0.0168(19) Uani 1 1 d .
Se2C Se 0.0034(7) 0.1559(3) -0.6075(6) 0.0130(17) Uani 1 1 d .
Se3A Se 0.8441(2) 0.35364(9) -0.2738(9) 0.0174(6) Uani 1 1 d .
Se3B Se 0.8437(7) 0.3568(3) 0.0667(7) 0.018(2) Uani 1 1 d .
Se3C Se 0.8427(7) 0.3563(3) 0.3856(7) 0.0138(18) Uani 1 1 d .
Se4A Se 0.1969(7) 0.0780(3) -0.4398(7) 0.016(2) Uani 1 1 d .
Se4B Se 0.1961(7) 0.0782(3) -0.1080(7) 0.0144(18) Uani 1 1 d .
Se4C Se 0.1953(2) 0.07437(10) 0.2250(10) 0.0204(7) Uani 1 1 d .
Se5A Se 0.7535(2) 0.23462(9) -0.2736(9) 0.0197(6) Uani 1 1 d .
Se5B Se 0.7765(7) 0.2371(3) 0.0661(7) 0.019(2) Uani 1 1 d .
Se5C Se 0.7776(7) 0.2379(3) 0.3868(7) 0.0152(19) Uani 1 1 d .
Se6A Se 0.8853(7) 0.0496(3) -0.4387(6) 0.023(2) Uani 1 1 d .
Se6B Se 0.8859(7) 0.0496(3) -0.1096(7) 0.0186(19) Uani 1 1 d .
Se6C Se 0.89019(19) 0.04558(9) 0.2268(9) 0.0184(6) Uani 1 1 d .
Se7A Se 0.3996(2) 0.00775(9) -0.2716(8) 0.0272(8) Uani 1 1 d .
Se7B Se 0.5942(8) -0.0060(3) -0.4503(7) 0.027(2) Uani 1 1 d .
Se7C Se 0.4041(8) 0.0059(3) -0.6088(7) 0.0272(19) Uani 1 1 d .
Se8A Se 0.03579(19) 0.27905(9) 0.2299(10) 0.0166(6) Uani 1 1 d .
Se8B Se 0.0424(7) 0.2804(3) -0.4766(6) 0.019(2) Uani 1 1 d .
Se8C Se 0.0428(7) 0.2803(3) -0.0630(7) 0.022(2) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sr Sr -1.5307 3.2498 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Y Y -2.7962 3.5667 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Se7A Sr1A Se1C 82.2(2) . 2_655
Se7A Sr1A Se1B 83.0(2) . .
Se1C Sr1A Se1B 84.19(9) 2_655 .
Se7A Sr1A Se3B 137.7(4) . 4_644
Se1C Sr1A Se3B 133.4(2) 2_655 4_644
Se1B Sr1A Se3B 79.9(3) . 4_644
Se7A Sr1A Se3C 136.9(4) . 4_644
Se1C Sr1A Se3C 80.1(3) 2_655 4_644
Se1B Sr1A Se3C 133.2(2) . 4_644
Se3B Sr1A Se3C 79.77(10) 4_644 4_644
Se7A Sr1A Se7C 62.1(2) . 2_655
Se1C Sr1A Se7C 87.2(3) 2_655 2_655
Se1B Sr1A Se7C 144.9(2) . 2_655
Se3B Sr1A Se7C 128.3(3) 4_644 2_655
Se3C Sr1A Se7C 78.0(3) 4_644 2_655
Se7A Sr1A Se7B 63.5(2) . .
Se1C Sr1A Se7B 145.2(2) 2_655 .
Se1B Sr1A Se7B 85.4(3) . .
Se3B Sr1A Se7B 76.7(3) 4_644 .
Se3C Sr1A Se7B 129.3(3) 4_644 .
Se7C Sr1A Se7B 82.46(11) 2_655 .
Se7A Sr1A Se4C 114.68(10) . 2_654
Se1C Sr1A Se4C 136.1(4) 2_655 2_654
Se1B Sr1A Se4C 135.6(4) . 2_654
Se3B Sr1A Se4C 59.4(2) 4_644 2_654
Se3C Sr1A Se4C 59.6(2) 4_644 2_654
Se7C Sr1A Se4C 69.1(2) 2_655 2_654
Se7B Sr1A Se4C 69.7(2) . 2_654
Se7A Sr1A Sr1C 92.5(3) . .
Se1C Sr1A Sr1C 131.9(3) 2_655 .
Se1B Sr1A Sr1C 47.8(2) . .
Se3B Sr1A Sr1C 48.2(3) 4_644 .
Se3C Sr1A Sr1C 128.0(3) 4_644 .
Se7C Sr1A Sr1C 131.8(3) 2_655 .
Se7B Sr1A Sr1C 49.4(2) . .
Se4C Sr1A Sr1C 89.4(3) 2_654 .
Se7A Sr1A Sr1B 92.8(3) . 2_655
Se1C Sr1A Sr1B 48.2(2) 2_655 2_655
Se1B Sr1A Sr1B 132.2(2) . 2_655
Se3B Sr1A Sr1B 126.9(2) 4_644 2_655
Se3C Sr1A Sr1B 47.2(2) 4_644 2_655
Se7C Sr1A Sr1B 52.2(2) 2_655 2_655
Se7B Sr1A Sr1B 134.5(2) . 2_655
Se4C Sr1A Sr1B 89.2(3) 2_654 2_655
Sr1C Sr1A Sr1B 174.60(11) . 2_655
Se7A Sr1A Y1B 92.8(3) . 2_655
Se1C Sr1A Y1B 48.2(2) 2_655 2_655
Se1B Sr1A Y1B 132.2(2) . 2_655
Se3B Sr1A Y1B 126.9(2) 4_644 2_655
Se3C Sr1A Y1B 47.2(2) 4_644 2_655
Se7C Sr1A Y1B 52.2(2) 2_655 2_655
Se7B Sr1A Y1B 134.5(2) . 2_655
Se4C Sr1A Y1B 89.2(3) 2_654 2_655
Sr1C Sr1A Y1B 174.60(11) . 2_655
Sr1B Sr1A Y1B 0.0(3) 2_655 2_655
Se3A Sr1B Se3C 88.3(3) 3_455 3_454
Se3A Sr1B Se1A 79.3(2) 3_455 .
Se3C Sr1B Se1A 139.7(3) 3_454 .
Se3A Sr1B Se1C 139.5(3) 3_455 .
Se3C Sr1B Se1C 79.8(3) 3_454 .
Se1A Sr1B Se1C 85.1(3) . .
Se3A Sr1B Se7B 135.5(3) 3_455 .
Se3C Sr1B Se7B 129.6(3) 3_454 .
Se1A Sr1B Se7B 82.2(3) . .
Se1C Sr1B Se7B 77.7(3) . .
Se3A Sr1B Se7A 77.0(2) 3_455 .
Se3C Sr1B Se7A 129.5(3) 3_454 .
Se1A Sr1B Se7A 85.0(2) . .
Se1C Sr1B Se7A 138.7(3) . .
Se7B Sr1B Se7A 61.2(2) . .
Se3A Sr1B Se7C 131.0(3) 3_455 .
Se3C Sr1B Se7C 76.3(3) 3_454 .
Se1A Sr1B Se7C 138.9(3) . .
Se1C Sr1B Se7C 83.6(3) . .
Se7B Sr1B Se7C 56.8(2) . .
Se7A Sr1B Se7C 78.1(3) . .
Se3A Sr1B Se4A 62.0(2) 3_455 .
Se3C Sr1B Se4A 62.0(2) 3_454 .
Se1A Sr1B Se4A 136.6(3) . .
Se1C Sr1B Se4A 137.2(3) . .
Se7B Sr1B Se4A 111.2(3) . .
Se7A Sr1B Se4A 68.5(2) . .
Se7C Sr1B Se4A 69.8(3) . .
Se3A Sr1B Se8B 74.1(2) 3_455 3
Se3C Sr1B Se8B 65.7(2) 3_454 3
Se1A Sr1B Se8B 74.0(2) . 3
Se1C Sr1B Se8B 65.7(2) . 3
Se7B Sr1B Se8B 137.4(3) . 3
Se7A Sr1B Se8B 146.8(3) . 3
Se7C Sr1B Se8B 134.1(3) . 3
Se4A Sr1B Se8B 110.4(3) . 3
Se3A Sr1B Sr1A 136.4(3) 3_455 2_654
Se3C Sr1B Sr1A 48.11(19) 3_454 2_654
Se1A Sr1B Sr1A 132.0(3) . 2_654
Se1C Sr1B Sr1A 46.93(19) . 2_654
Se7B Sr1B Sr1A 84.6(2) . 2_654
Se7A Sr1B Sr1A 126.9(3) . 2_654
Se7C Sr1B Sr1A 48.83(17) . 2_654
Se4A Sr1B Sr1A 91.1(2) . 2_654
Se8B Sr1B Sr1A 85.82(19) 3 2_654
Se3A Sr1B Y1A 136.4(3) 3_455 2_654
Se3C Sr1B Y1A 48.11(19) 3_454 2_654
Se1A Sr1B Y1A 132.0(3) . 2_654
Se1C Sr1B Y1A 46.93(19) . 2_654
Se7B Sr1B Y1A 84.6(2) . 2_654
Se7A Sr1B Y1A 126.9(3) . 2_654
Se7C Sr1B Y1A 48.83(17) . 2_654
Se4A Sr1B Y1A 91.1(2) . 2_654
Se8B Sr1B Y1A 85.82(19) 3 2_654
Sr1A Sr1B Y1A 0.00(7) 2_654 2_654
Se3A Sr1B Sr1C 47.9(2) 3_455 2_655
Se3C Sr1B Sr1C 136.2(4) 3_454 2_655
Se1A Sr1B Sr1C 47.1(2) . 2_655
Se1C Sr1B Sr1C 132.1(4) . 2_655
Se7B Sr1B Sr1C 90.8(3) . 2_655
Se7A Sr1B Sr1C 50.0(2) . 2_655
Se7C Sr1B Sr1C 128.0(3) . 2_655
Se4A Sr1B Sr1C 90.4(3) . 2_655
Se8B Sr1B Sr1C 97.7(3) 3 2_655
Sr1A Sr1B Sr1C 175.4(3) 2_654 2_655
Y1A Sr1B Sr1C 175.4(3) 2_654 2_655
Se1A Sr1C Se7C 82.1(3) 2_654 .
Se1A Sr1C Se1B 86.2(3) 2_654 .
Se7C Sr1C Se1B 81.1(3) . .
Se1A Sr1C Se3A 78.4(3) 2_654 4_644
Se7C Sr1C Se3A 134.3(4) . 4_644
Se1B Sr1C Se3A 137.3(4) . 4_644
Se1A Sr1C Se3B 137.7(4) 2_654 4_644
Se7C Sr1C Se3B 133.1(4) . 4_644
Se1B Sr1C Se3B 79.1(3) . 4_644
Se3A Sr1C Se3B 86.1(3) 4_644 4_644
Se1A Sr1C Se7B 141.1(4) 2_654 .
Se7C Sr1C Se7B 59.1(2) . .
Se1B Sr1C Se7B 86.0(3) . .
Se3A Sr1C Se7B 129.4(3) 4_644 .
Se3B Sr1C Se7B 77.4(3) 4_644 .
Se1A Sr1C Se7A 86.4(3) 2_654 2_654
Se7C Sr1C Se7A 60.6(2) . 2_654
Se1B Sr1C Se7A 141.6(4) . 2_654
Se3A Sr1C Se7A 77.2(2) 4_644 2_654
Se3B Sr1C Se7A 128.2(3) 4_644 2_654
Se7B Sr1C Se7A 76.6(3) . 2_654
Se1A Sr1C Se4B 135.1(3) 2_654 2_654
Se7C Sr1C Se4B 112.8(3) . 2_654
Se1B Sr1C Se4B 136.3(4) . 2_654
Se3A Sr1C Se4B 60.7(2) 4_644 2_654
Se3B Sr1C Se4B 60.9(3) 4_644 2_654
Se7B Sr1C Se4B 69.6(3) . 2_654
Se7A Sr1C Se4B 68.2(2) 2_654 2_654
Se1A Sr1C Sr1A 133.3(3) 2_654 .
Se7C Sr1C Sr1A 88.5(3) . .
Se1B Sr1C Sr1A 47.1(2) . .
Se3A Sr1C Sr1A 133.9(3) 4_644 .
Se3B Sr1C Sr1A 47.8(2) 4_644 .
Se7B Sr1C Sr1A 50.85(19) . .
Se7A Sr1C Sr1A 127.5(3) 2_654 .
Se4B Sr1C Sr1A 90.6(2) 2_654 .
Se1A Sr1C Y1B 47.2(2) 2_654 2_654
Se7C Sr1C Y1B 90.8(3) . 2_654
Se1B Sr1C Y1B 133.4(4) . 2_654
Se3A Sr1C Y1B 46.5(2) 4_644 2_654
Se3B Sr1C Y1B 132.6(4) 4_644 2_654
Se7B Sr1C Y1B 128.2(4) . 2_654
Se7A Sr1C Y1B 51.6(2) 2_654 2_654
Se4B Sr1C Y1B 89.1(3) 2_654 2_654
Sr1A Sr1C Y1B 179.0(4) . 2_654
Se1A Sr1C Sr1B 47.2(2) 2_654 2_654
Se7C Sr1C Sr1B 90.8(3) . 2_654
Se1B Sr1C Sr1B 133.4(4) . 2_654
Se3A Sr1C Sr1B 46.5(2) 4_644 2_654
Se3B Sr1C Sr1B 132.6(4) 4_644 2_654
Se7B Sr1C Sr1B 128.2(4) . 2_654
Se7A Sr1C Sr1B 51.6(2) 2_654 2_654
Se4B Sr1C Sr1B 89.1(3) 2_654 2_654
Sr1A Sr1C Sr1B 179.0(4) . 2_654
Y1B Sr1C Sr1B 0.0(2) 2_654 2_654
Se1C Sr2A Se1B 82.69(9) 1_556 2_655
Se1C Sr2A Se2C 93.8(4) 1_556 1_656
Se1B Sr2A Se2C 159.3(2) 2_655 1_656
Se1C Sr2A Se2B 159.3(2) 1_556 1_655
Se1B Sr2A Se2B 93.4(4) 2_655 1_655
Se2C Sr2A Se2B 82.72(8) 1_656 1_655
Se1C Sr2A Se5B 127.1(2) 1_556 .
Se1B Sr2A Se5B 76.2(3) 2_655 .
Se2C Sr2A Se5B 120.8(2) 1_656 .
Se2B Sr2A Se5B 70.8(3) 1_655 .
Se1C Sr2A Se5C 76.8(3) 1_556 .
Se1B Sr2A Se5C 127.4(2) 2_655 .
Se2C Sr2A Se5C 70.8(3) 1_656 .
Se2B Sr2A Se5C 120.5(2) 1_655 .
Se5B Sr2A Se5C 78.83(8) . .
Se1C Sr2A Se6C 80.7(2) 1_556 .
Se1B Sr2A Se6C 80.8(2) 2_655 .
Se2C Sr2A Se6C 78.6(2) 1_656 .
Se2B Sr2A Se6C 78.6(2) 1_655 .
Se5B Sr2A Se6C 140.1(4) . .
Se5C Sr2A Se6C 140.2(4) . .
Se1C Sr2A Sr2C 130.9(3) 1_556 .
Se1B Sr2A Sr2C 48.2(3) 2_655 .
Se2C Sr2A Sr2C 132.3(2) 1_656 .
Se2B Sr2A Sr2C 49.6(2) 1_655 .
Se5B Sr2A Sr2C 49.0(2) . .
Se5C Sr2A Sr2C 127.8(2) . .
Se6C Sr2A Sr2C 91.6(3) . .
Se1C Sr2A Sr2B 48.5(3) 1_556 1_556
Se1B Sr2A Sr2B 131.2(3) 2_655 1_556
Se2C Sr2A Sr2B 49.6(2) 1_656 1_556
Se2B Sr2A Sr2B 132.3(3) 1_655 1_556
Se5B Sr2A Sr2B 128.4(3) . 1_556
Se5C Sr2A Sr2B 49.6(2) . 1_556
Se6C Sr2A Sr2B 91.1(3) . 1_556
Sr2C Sr2A Sr2B 177.03(9) . 1_556
Se1C Sr2A Y2B 48.5(3) 1_556 1_556
Se1B Sr2A Y2B 131.2(3) 2_655 1_556
Se2C Sr2A Y2B 49.6(2) 1_656 1_556
Se2B Sr2A Y2B 132.3(3) 1_655 1_556
Se5B Sr2A Y2B 128.4(3) . 1_556
Se5C Sr2A Y2B 49.6(2) . 1_556
Se6C Sr2A Y2B 91.1(3) . 1_556
Sr2C Sr2A Y2B 177.03(9) . 1_556
Sr2B Sr2A Y2B 0.0(2) 1_556 1_556
Se1C Sr2A Sr3A 135.5(4) 1_556 1_655
Se1B Sr2A Sr3A 135.1(4) 2_655 1_655
Se2C Sr2A Sr3A 42.2(2) 1_656 1_655
Se2B Sr2A Sr3A 42.1(2) 1_655 1_655
Se5B Sr2A Sr3A 90.2(2) . 1_655
Se5C Sr2A Sr3A 90.0(2) . 1_655
Se6C Sr2A Sr3A 83.63(7) . 1_655
Sr2C Sr2A Sr3A 90.7(2) . 1_655
Sr2B Sr2A Sr3A 90.8(2) 1_556 1_655
Y2B Sr2A Sr3A 90.8(2) 1_556 1_655
Se1A Sr2B Se1C 84.3(3) . .
Se1A Sr2B Se6A 80.7(3) . .
Se1C Sr2B Se6A 79.7(3) . .
Se1A Sr2B Se5A 71.1(2) . .
Se1C Sr2B Se5A 126.1(3) . .
Se6A Sr2B Se5A 137.9(3) . .
Se1A Sr2B Se2A 94.1(3) . 1_655
Se1C Sr2B Se2A 158.5(3) . 1_655
Se6A Sr2B Se2A 78.9(3) . 1_655
Se5A Sr2B Se2A 72.8(2) . 1_655
Se1A Sr2B Se2C 158.0(3) . 1_655
Se1C Sr2B Se2C 92.1(3) . 1_655
Se6A Sr2B Se2C 77.3(3) . 1_655
Se5A Sr2B Se2C 126.7(3) . 1_655
Se2A Sr2B Se2C 81.4(3) 1_655 1_655
Se1A Sr2B Se5C 129.7(3) . 1_554
Se1C Sr2B Se5C 75.8(3) . 1_554
Se6A Sr2B Se5C 137.5(3) . 1_554
Se5A Sr2B Se5C 84.2(3) . 1_554
Se2A Sr2B Se5C 120.0(3) 1_655 1_554
Se2C Sr2B Se5C 69.6(3) 1_655 1_554
Se1A Sr2B Y2A 132.2(3) . 1_554
Se1C Sr2B Y2A 47.84(19) . 1_554
Se6A Sr2B Y2A 89.3(2) . 1_554
Se5A Sr2B Y2A 132.8(3) . 1_554
Se2A Sr2B Y2A 129.8(3) 1_655 1_554
Se2C Sr2B Y2A 48.43(18) 1_655 1_554
Se5C Sr2B Y2A 48.79(18) 1_554 1_554
Se1A Sr2B Sr2A 132.2(3) . 1_554
Se1C Sr2B Sr2A 47.84(19) . 1_554
Se6A Sr2B Sr2A 89.3(2) . 1_554
Se5A Sr2B Sr2A 132.8(3) . 1_554
Se2A Sr2B Sr2A 129.8(3) 1_655 1_554
Se2C Sr2B Sr2A 48.43(18) 1_655 1_554
Se5C Sr2B Sr2A 48.79(18) 1_554 1_554
Y2A Sr2B Sr2A 0.00(6) 1_554 1_554
Se1A Sr2B Sr2C 48.1(2) . .
Se1C Sr2B Sr2C 132.4(4) . .
Se6A Sr2B Sr2C 89.9(3) . .
Se5A Sr2B Sr2C 48.0(2) . .
Se2A Sr2B Sr2C 49.5(2) 1_655 .
Se2C Sr2B Sr2C 130.9(4) 1_655 .
Se5C Sr2B Sr2C 132.0(4) 1_554 .
Y2A Sr2B Sr2C 179.0(4) 1_554 .
Sr2A Sr2B Sr2C 179.0(4) 1_554 .
Se1A Sr2B Sr1B 42.4(2) . .
Se1C Sr2B Sr1B 43.2(2) . .
Se6A Sr2B Sr1B 84.8(3) . .
Se5A Sr2B Sr1B 94.2(2) . .
Se2A Sr2B Sr1B 135.7(3) 1_655 .
Se2C Sr2B Sr1B 134.5(3) 1_655 .
Se5C Sr2B Sr1B 99.7(3) 1_554 .
Y2A Sr2B Sr1B 90.39(18) 1_554 .
Sr2A Sr2B Sr1B 90.39(18) 1_554 .
Sr2C Sr2B Sr1B 90.0(3) . .
Se1B Sr2C Se1A 84.8(3) 2_655 .
Se1B Sr2C Se5A 126.8(3) 2_655 .
Se1A Sr2C Se5A 70.8(2) . .
Se1B Sr2C Se5B 75.9(3) 2_655 .
Se1A Sr2C Se5B 130.4(3) . .
Se5A Sr2C Se5B 85.1(3) . .
Se1B Sr2C Se6B 79.8(3) 2_655 .
Se1A Sr2C Se6B 80.1(2) . .
Se5A Sr2C Se6B 136.8(4) . .
Se5B Sr2C Se6B 137.7(4) . .
Se1B Sr2C Se2B 92.3(3) 2_655 1_655
Se1A Sr2C Se2B 157.1(3) . 1_655
Se5A Sr2C Se2B 127.0(3) . 1_655
Se5B Sr2C Se2B 70.0(3) . 1_655
Se6B Sr2C Se2B 77.0(3) . 1_655
Se1B Sr2C Se2A 157.8(3) 2_655 1_655
Se1A Sr2C Se2A 92.6(3) . 1_655
Se5A Sr2C Se2A 72.2(2) . 1_655
Se5B Sr2C Se2A 120.9(3) . 1_655
Se6B Sr2C Se2A 78.1(2) . 1_655
Se2B Sr2C Se2A 81.6(3) 1_655 1_655
Se1B Sr2C Sr2A 48.1(2) 2_655 .
Se1A Sr2C Sr2A 132.8(3) . .
Se5A Sr2C Sr2A 133.7(3) . .
Se5B Sr2C Sr2A 48.8(2) . .
Se6B Sr2C Sr2A 89.5(2) . .
Se2B Sr2C Sr2A 48.6(2) 1_655 .
Se2A Sr2C Sr2A 130.2(3) 1_655 .
Se1B Sr2C Sr2B 132.2(4) 2_655 .
Se1A Sr2C Sr2B 47.5(2) . .
Se5A Sr2C Sr2B 48.2(2) . .
Se5B Sr2C Sr2B 132.9(4) . .
Se6B Sr2C Sr2B 88.7(3) . .
Se2B Sr2C Sr2B 130.1(4) 1_655 .
Se2A Sr2C Sr2B 48.6(2) 1_655 .
Sr2A Sr2C Sr2B 178.0(3) . .
Se1B Sr2C Sr1C 43.1(2) 2_655 2_655
Se1A Sr2C Sr1C 42.7(2) . 2_655
Se5A Sr2C Sr1C 95.2(2) . 2_655
Se5B Sr2C Sr1C 100.8(3) . 2_655
Se6B Sr2C Sr1C 83.6(3) . 2_655
Se2B Sr2C Sr1C 134.2(3) 1_655 2_655
Se2A Sr2C Sr1C 134.2(3) 1_655 2_655
Sr2A Sr2C Sr1C 90.72(19) . 2_655
Sr2B Sr2C Sr1C 89.8(3) . 2_655
Se2B Sr3A Se2C 85.39(9) . 1_556
Se2B Sr3A Se4C 78.9(2) . .
Se2C Sr3A Se4C 79.2(3) 1_556 .
Se2B Sr3A Se3C 144.1(2) . 3_455
Se2C Sr3A Se3C 86.7(3) 1_556 3_455
Se4C Sr3A Se3C 65.3(2) . 3_455
Se2B Sr3A Se3B 87.1(3) . 3_455
Se2C Sr3A Se3B 144.0(2) 1_556 3_455
Se4C Sr3A Se3B 64.8(2) . 3_455
Se3C Sr3A Se3B 79.14(8) 3_455 3_455
Se2B Sr3A Se8A 81.8(2) . .
Se2C Sr3A Se8A 80.6(2) 1_556 .
Se4C Sr3A Se8A 153.01(11) . .
Se3C Sr3A Se8A 131.0(4) 3_455 .
Se3B Sr3A Se8A 132.9(4) 3_455 .
Se2B Sr3A Se5B 92.1(3) . 3_455
Se2C Sr3A Se5B 149.5(2) 1_556 3_455
Se4C Sr3A Se5B 130.2(4) . 3_455
Se3C Sr3A Se5B 111.5(2) 3_455 3_455
Se3B Sr3A Se5B 65.9(3) 3_455 3_455
Se8A Sr3A Se5B 69.0(2) . 3_455
Se2B Sr3A Se5C 150.0(2) . 3_455
Se2C Sr3A Se5C 91.8(3) 1_556 3_455
Se4C Sr3A Se5C 129.9(4) . 3_455
Se3C Sr3A Se5C 65.1(3) 3_455 3_455
Se3B Sr3A Se5C 111.3(2) 3_455 3_455
Se8A Sr3A Se5C 68.2(2) . 3_455
Se5B Sr3A Se5C 75.45(8) 3_455 3_455
Se2B Sr3A Sr3C 48.6(2) . .
Se2C Sr3A Sr3C 134.0(2) 1_556 .
Se4C Sr3A Sr3C 91.1(3) . .
Se3C Sr3A Sr3C 129.7(3) 3_455 .
Se3B Sr3A Sr3C 50.6(3) 3_455 .
Se8A Sr3A Sr3C 90.2(3) . .
Se5B Sr3A Sr3C 50.9(2) 3_455 .
Se5C Sr3A Sr3C 126.4(2) 3_455 .
Se2B Sr3A Y3B 133.6(3) . 1_556
Se2C Sr3A Y3B 48.2(2) 1_556 1_556
Se4C Sr3A Y3B 91.4(3) . 1_556
Se3C Sr3A Y3B 50.3(2) 3_455 1_556
Se3B Sr3A Y3B 129.4(3) 3_455 1_556
Se8A Sr3A Y3B 88.3(3) . 1_556
Se5B Sr3A Y3B 126.1(3) 3_455 1_556
Se5C Sr3A Y3B 50.6(2) 3_455 1_556
Sr3C Sr3A Y3B 177.00(9) . 1_556
Se2B Sr3A Sr3B 133.6(3) . 1_556
Se2C Sr3A Sr3B 48.2(2) 1_556 1_556
Se4C Sr3A Sr3B 91.4(3) . 1_556
Se3C Sr3A Sr3B 50.3(2) 3_455 1_556
Se3B Sr3A Sr3B 129.4(3) 3_455 1_556
Se8A Sr3A Sr3B 88.3(3) . 1_556
Se5B Sr3A Sr3B 126.1(3) 3_455 1_556
Se5C Sr3A Sr3B 50.6(2) 3_455 1_556
Sr3C Sr3A Sr3B 177.00(9) . 1_556
Y3B Sr3A Sr3B 0.000(6) 1_556 1_556
Se4A Sr3B Se2C 77.6(3) . .
Se4A Sr3B Se2A 79.1(3) . .
Se2C Sr3B Se2A 83.8(3) . .
Se4A Sr3B Se8B 151.7(4) . .
Se2C Sr3B Se8B 77.2(3) . .
Se2A Sr3B Se8B 85.6(3) . .
Se4A Sr3B Se3A 65.2(2) . 3_455
Se2C Sr3B Se3A 142.6(3) . 3_455
Se2A Sr3B Se3A 85.9(3) . 3_455
Se8B Sr3B Se3A 137.6(3) . 3_455
Se4A Sr3B Se5A 131.1(3) . 3_455
Se2C Sr3B Se5A 147.0(3) . 3_455
Se2A Sr3B Se5A 86.3(3) . 3_455
Se8B Sr3B Se5A 70.6(2) . 3_455
Se3A Sr3B Se5A 67.4(2) 3_455 3_455
Se4A Sr3B Se3C 65.0(3) . 3_454
Se2C Sr3B Se3C 84.2(3) . 3_454
Se2A Sr3B Se3C 143.8(3) . 3_454
Se8B Sr3B Se3C 124.6(3) . 3_454
Se3A Sr3B Se3C 83.2(3) 3_455 3_454
Se5A Sr3B Se3C 120.3(3) 3_455 3_454
Se4A Sr3B Se5C 128.6(3) . 3_454
Se2C Sr3B Se5C 91.1(3) . 3_454
Se2A Sr3B Se5C 150.1(3) . 3_454
Se8B Sr3B Se5C 64.6(3) . 3_454
Se3A Sr3B Se5C 114.2(3) 3_455 3_454
Se5A Sr3B Se5C 82.0(3) 3_455 3_454
Se3C Sr3B Se5C 64.1(2) 3_454 3_454
Se4A Sr3B Bi4B 101.3(3) . 3_455
Se2C Sr3B Bi4B 169.1(3) . 3_455
Se2A Sr3B Bi4B 106.7(2) . 3_455
Se8B Sr3B Bi4B 105.8(3) . 3_455
Se3A Sr3B Bi4B 38.82(11) 3_455 3_455
Se5A Sr3B Bi4B 39.65(11) 3_455 3_455
Se3C Sr3B Bi4B 85.5(2) 3_454 3_455
Se5C Sr3B Bi4B 81.1(2) 3_454 3_455
Se4A Sr3B Sr3A 89.4(2) . 1_554
Se2C Sr3B Sr3A 47.38(19) . 1_554
Se2A Sr3B Sr3A 131.2(3) . 1_554
Se8B Sr3B Sr3A 83.0(2) . 1_554
Se3A Sr3B Sr3A 131.3(3) 3_455 1_554
Se5A Sr3B Sr3A 132.5(3) 3_455 1_554
Se3C Sr3B Sr3A 48.19(18) 3_454 1_554
Se5C Sr3B Sr3A 50.73(19) 3_454 1_554
Bi4B Sr3B Sr3A 122.0(2) 3_455 1_554
Se4A Sr3B Y3A 89.4(2) . 1_554
Se2C Sr3B Y3A 47.38(19) . 1_554
Se2A Sr3B Y3A 131.2(3) . 1_554
Se8B Sr3B Y3A 83.0(2) . 1_554
Se3A Sr3B Y3A 131.3(3) 3_455 1_554
Se5A Sr3B Y3A 132.5(3) 3_455 1_554
Se3C Sr3B Y3A 48.19(18) 3_454 1_554
Se5C Sr3B Y3A 50.73(19) 3_454 1_554
Bi4B Sr3B Y3A 122.0(2) 3_455 1_554
Sr3A Sr3B Y3A 0.000(8) 1_554 1_554
Se4B Sr3C Se2B 77.6(3) . .
Se4B Sr3C Se2A 78.7(3) . .
Se2B Sr3C Se2A 84.1(3) . .
Se4B Sr3C Se8C 151.0(4) . .
Se2B Sr3C Se8C 76.2(3) . .
Se2A Sr3C Se8C 86.6(3) . .
Se4B Sr3C Se3A 65.2(2) . 3_455
Se2B Sr3C Se3A 142.6(3) . 3_455
Se2A Sr3C Se3A 85.1(3) . 3_455
Se8C Sr3C Se3A 138.6(3) . 3_455
Se4B Sr3C Se5A 130.8(4) . 3_455
Se2B Sr3C Se5A 146.7(3) . 3_455
Se2A Sr3C Se5A 85.5(3) . 3_455
Se8C Sr3C Se5A 71.8(3) . 3_455
Se3A Sr3C Se5A 67.2(2) 3_455 3_455
Se4B Sr3C Se3B 65.2(3) . 3_455
Se2B Sr3C Se3B 84.8(3) . 3_455
Se2A Sr3C Se3B 143.7(3) . 3_455
Se8C Sr3C Se3B 123.7(3) . 3_455
Se3A Sr3C Se3B 83.2(3) 3_455 3_455
Se5A Sr3C Se3B 120.6(3) 3_455 3_455
Se4B Sr3C Se5B 129.7(4) . 3_455
Se2B Sr3C Se5B 91.4(3) . 3_455
Se2A Sr3C Se5B 149.6(3) . 3_455
Se8C Sr3C Se5B 63.1(3) . 3_455
Se3A Sr3C Se5B 114.8(3) 3_455 3_455
Se5A Sr3C Se5B 82.0(3) 3_455 3_455
Se3B Sr3C Se5B 65.0(3) 3_455 3_455
Se4B Sr3C Bi4B 101.4(3) . 3_455
Se2B Sr3C Bi4B 169.3(3) . 3_455
Se2A Sr3C Bi4B 106.3(3) . 3_455
Se8C Sr3C Bi4B 106.6(3) . 3_455
Se3A Sr3C Bi4B 39.03(11) 3_455 3_455
Se5A Sr3C Bi4B 39.85(11) 3_455 3_455
Se3B Sr3C Bi4B 85.2(3) 3_455 3_455
Se5B Sr3C Bi4B 81.0(2) 3_455 3_455
Se4B Sr3C Sr3A 89.8(3) . .
Se2B Sr3C Sr3A 47.6(2) . .
Se2A Sr3C Sr3A 131.7(3) . .
Se8C Sr3C Sr3A 81.5(2) . .
Se3A Sr3C Sr3A 131.8(3) 3_455 .
Se5A Sr3C Sr3A 132.9(3) 3_455 .
Se3B Sr3C Sr3A 48.68(19) 3_455 .
Se5B Sr3C Sr3A 51.09(19) 3_455 .
Bi4B Sr3C Sr3A 122.0(2) 3_455 .
Se8C Ge4A Se3B 108.0(5) 1_655 .
Se8C Ge4A Se5B 117.5(5) 1_655 .
Se3B Ge4A Se5B 98.8(5) . .
Se8C Ge4A Se8A 104.3(5) 1_655 1_655
Se3B Ge4A Se8A 110.4(4) . 1_655
Se5B Ge4A Se8A 117.5(4) . 1_655
Se3A Bi4B Se5A 85.64(8) . .
Se3A Bi4B Se8B 98.2(3) . 1_655
Se5A Bi4B Se8B 114.3(3) . 1_655
Se3A Bi4B Se8C 99.0(3) . 1_655
Se5A Bi4B Se8C 114.6(3) . 1_655
Se8B Bi4B Se8C 129.05(8) 1_655 1_655
Se3A Bi4B Sr3C 51.0(2) . 3
Se5A Bi4B Sr3C 51.5(2) . 3
Se8B Bi4B Sr3C 142.5(2) 1_655 3
Se8C Bi4B Sr3C 82.1(2) 1_655 3
Se3A Bi4B Sr3B 50.5(2) . 3
Se5A Bi4B Sr3B 51.1(2) . 3
Se8B Bi4B Sr3B 82.3(2) 1_655 3
Se8C Bi4B Sr3B 142.3(2) 1_655 3
Sr3C Bi4B Sr3B 61.88(5) 3 3
Se5C Ge4C Se3C 98.1(5) . .
Se5C Ge4C Se8B 117.8(5) . 1_656
Se3C Ge4C Se8B 108.6(5) . 1_656
Se5C Ge4C Se8A 117.3(4) . 1_655
Se3C Ge4C Se8A 109.9(4) . 1_655
Se8B Ge4C Se8A 104.7(4) 1_656 1_655
Se2A Bi5A Se4B 93.0(2) . .
Se2A Bi5A Se4A 92.5(3) . .
Se4B Bi5A Se4A 97.89(8) . .
Se2A Bi5A Se6B 90.0(2) . 1_455
Se4B Bi5A Se6B 87.4(3) . 1_455
Se4A Bi5A Se6B 174.0(3) . 1_455
Se2A Bi5A Se6A 89.4(2) . 1_455
Se4B Bi5A Se6A 174.1(3) . 1_455
Se4A Bi5A Se6A 87.4(3) . 1_455
Se6B Bi5A Se6A 87.18(8) 1_455 1_455
Se2B Bi5B Se4C 93.0(2) . .
Se2B Bi5B Se4B 91.6(3) . .
Se4C Bi5B Se4B 98.4(3) . .
Se2B Bi5B Se6C 90.4(2) . 1_455
Se4C Bi5B Se6C 85.5(2) . 1_455
Se4B Bi5B Se6C 175.6(3) . 1_455
Se2B Bi5B Se6B 88.7(3) . 1_455
Se4C Bi5B Se6B 174.6(3) . 1_455
Se4B Bi5B Se6B 86.8(3) . 1_455
Se6C Bi5B Se6B 89.3(2) 1_455 1_455
Se2C Bi5C Se4A 91.8(3) . .
Se2C Bi5C Se4C 92.7(2) . 1_554
Se4A Bi5C Se4C 98.5(2) . 1_554
Se2C Bi5C Se6C 90.3(2) . 1_454
Se4A Bi5C Se6C 175.7(3) . 1_454
Se4C Bi5C Se6C 85.1(2) 1_554 1_454
Se2C Bi5C Se6A 88.9(3) . 1_455
Se4A Bi5C Se6A 87.4(3) . 1_455
Se4C Bi5C Se6A 173.8(3) 1_554 1_455
Se6C Bi5C Se6A 88.9(2) 1_454 1_455
Se1A Bi6A Se7C 94.1(3) . 2_655
Se1A Bi6A Se6A 92.8(3) . .
Se7C Bi6A Se6A 173.0(3) 2_655 .
Se1A Bi6A Se6B 93.2(2) . .
Se7C Bi6A Se6B 87.3(3) 2_655 .
Se6A Bi6A Se6B 90.95(8) . .
Se1A Bi6A Se7B 93.5(3) . .
Se7C Bi6A Se7B 95.30(10) 2_655 .
Se6A Bi6A Se7B 85.6(3) . .
Se6B Bi6A Se7B 172.6(3) . .
Se1A Bi6A Se4C 174.83(9) . 2_654
Se7C Bi6A Se4C 82.7(3) 2_655 2_654
Se6A Bi6A Se4C 90.5(3) . 2_654
Se6B Bi6A Se4C 90.8(2) . 2_654
Se7B Bi6A Se4C 82.7(3) . 2_654
Se1B Bi6B Se7A 94.1(2) . .
Se1B Bi6B Se7C 92.6(3) . .
Se7A Bi6B Se7C 95.5(3) . .
Se1B Bi6B Se6C 93.6(2) . 2_654
Se7A Bi6B Se6C 86.6(2) . 2_654
Se7C Bi6B Se6C 173.3(3) . 2_654
Se1B Bi6B Se6B 91.1(3) . 2_654
Se7A Bi6B Se6B 174.7(2) . 2_654
Se7C Bi6B Se6B 85.2(3) . 2_654
Se6C Bi6B Se6B 92.0(2) 2_654 2_654
Se1B Bi6B Se4A 174.2(3) . .
Se7A Bi6B Se4A 82.37(19) . .
Se7C Bi6B Se4A 83.2(3) . .
Se6C Bi6B Se4A 90.8(2) 2_654 .
Se6B Bi6B Se4A 92.5(2) 2_654 .
Se1C Bi6C Se7A 93.9(2) . 2_654
Se1C Bi6C Se7B 92.5(3) . .
Se7A Bi6C Se7B 92.5(3) 2_654 .
Se1C Bi6C Se6C 93.5(2) . 1_554
Se7A Bi6C Se6C 87.5(2) 2_654 1_554
Se7B Bi6C Se6C 173.9(2) . 1_554
Se1C Bi6C Se6A 91.1(3) . .
Se7A Bi6C Se6A 174.9(2) 2_654 .
Se7B Bi6C Se6A 87.7(3) . .
Se6C Bi6C Se6A 91.7(2) 1_554 .
Se1C Bi6C Se4B 174.3(3) . 2_654
Se7A Bi6C Se4B 82.34(19) 2_654 2_654
Se7B Bi6C Se4B 83.3(3) . 2_654
Se6C Bi6C Se4B 90.7(2) 1_554 2_654
Se6A Bi6C Se4B 92.7(3) . 2_654
Bi6A Se1A Y1C 93.3(3) . 2_655
Bi6A Se1A Sr1C 93.3(3) . 2_655
Y1C Se1A Sr1C 0.0(5) 2_655 2_655
Bi6A Se1A Sr1B 95.3(2) . .
Y1C Se1A Sr1B 85.74(9) 2_655 .
Sr1C Se1A Sr1B 85.74(9) 2_655 .
Bi6A Se1A Sr2B 95.4(3) . .
Y1C Se1A Sr2B 171.3(3) 2_655 .
Sr1C Se1A Sr2B 171.3(3) 2_655 .
Sr1B Se1A Sr2B 94.7(4) . .
Bi6A Se1A Sr2C 95.5(2) . .
Y1C Se1A Sr2C 93.5(4) 2_655 .
Sr1C Se1A Sr2C 93.5(4) 2_655 .
Sr1B Se1A Sr2C 169.2(2) . .
Sr2B Se1A Sr2C 84.44(9) . .
Bi6B Se1B Sr1A 92.0(3) . .
Bi6B Se1B Sr1C 94.8(3) . .
Sr1A Se1B Sr1C 85.1(3) . .
Bi6B Se1B Y2A 95.5(3) . 2_654
Sr1A Se1B Y2A 96.0(3) . 2_654
Sr1C Se1B Y2A 169.6(3) . 2_654
Bi6B Se1B Sr2A 95.5(3) . 2_654
Sr1A Se1B Sr2A 96.0(3) . 2_654
Sr1C Se1B Sr2A 169.6(3) . 2_654
Y2A Se1B Sr2A 0.0(3) 2_654 2_654
Bi6B Se1B Y2C 97.6(3) . 2_654
Sr1A Se1B Y2C 170.3(3) . 2_654
Sr1C Se1B Y2C 93.5(3) . 2_654
Y2A Se1B Y2C 83.7(3) 2_654 2_654
Sr2A Se1B Y2C 83.7(3) 2_654 2_654
Bi6B Se1B Sr2C 97.6(3) . 2_654
Sr1A Se1B Sr2C 170.3(3) . 2_654
Sr1C Se1B Sr2C 93.5(3) . 2_654
Y2A Se1B Sr2C 83.7(3) 2_654 2_654
Sr2A Se1B Sr2C 83.7(3) 2_654 2_654
Y2C Se1B Sr2C 0.0(3) 2_654 2_654
Bi6C Se1C Y1A 92.2(3) . 2_654
Bi6C Se1C Sr1A 92.2(3) . 2_654
Y1A Se1C Sr1A 0.0(3) 2_654 2_654
Bi6C Se1C Y2A 95.6(3) . 1_554
Y1A Se1C Y2A 96.2(3) 2_654 1_554
Sr1A Se1C Y2A 96.2(3) 2_654 1_554
Bi6C Se1C Sr2A 95.6(3) . 1_554
Y1A Se1C Sr2A 96.2(3) 2_654 1_554
Sr1A Se1C Sr2A 96.2(3) 2_654 1_554
Y2A Se1C Sr2A 0.00(10) 1_554 1_554
Bi6C Se1C Sr1B 96.5(3) . .
Y1A Se1C Sr1B 84.9(3) 2_654 .
Sr1A Se1C Sr1B 84.9(3) 2_654 .
Y2A Se1C Sr1B 167.8(3) 1_554 .
Sr2A Se1C Sr1B 167.8(3) 1_554 .
Bi6C Se1C Sr2B 97.0(3) . .
Y1A Se1C Sr2B 170.8(4) 2_654 .
Sr1A Se1C Sr2B 170.8(4) 2_654 .
Y2A Se1C Sr2B 83.7(3) 1_554 .
Sr2A Se1C Sr2B 83.7(3) 1_554 .
Sr1B Se1C Sr2B 93.3(3) . .
Bi5A Se2A Sr3B 94.1(2) . .
Bi5A Se2A Sr3C 93.5(2) . .
Sr3B Se2A Sr3C 85.13(8) . .
Bi5A Se2A Y2B 98.3(2) . 1_455
Sr3B Se2A Y2B 95.9(3) . 1_455
Sr3C Se2A Y2B 168.1(2) . 1_455
Bi5A Se2A Sr2B 98.3(2) . 1_455
Sr3B Se2A Sr2B 95.9(3) . 1_455
Sr3C Se2A Sr2B 168.1(2) . 1_455
Y2B Se2A Sr2B 0.0(3) 1_455 1_455
Bi5A Se2A Y2C 98.0(2) . 1_455
Sr3B Se2A Y2C 167.9(2) . 1_455
Sr3C Se2A Y2C 94.6(3) . 1_455
Y2B Se2A Y2C 81.91(8) 1_455 1_455
Sr2B Se2A Y2C 81.91(8) 1_455 1_455
Bi5A Se2A Sr2C 98.0(2) . 1_455
Sr3B Se2A Sr2C 167.9(2) . 1_455
Sr3C Se2A Sr2C 94.6(3) . 1_455
Y2B Se2A Sr2C 81.91(8) 1_455 1_455
Sr2B Se2A Sr2C 81.91(8) 1_455 1_455
Y2C Se2A Sr2C 0.0(2) 1_455 1_455
Bi5B Se2B Sr3A 95.1(3) . .
Bi5B Se2B Sr3C 95.8(3) . .
Sr3A Se2B Sr3C 83.7(3) . .
Bi5B Se2B Y2A 99.2(3) . 1_455
Sr3A Se2B Y2A 94.4(3) . 1_455
Sr3C Se2B Y2A 165.0(3) . 1_455
Bi5B Se2B Sr2A 99.2(3) . 1_455
Sr3A Se2B Sr2A 94.4(3) . 1_455
Sr3C Se2B Sr2A 165.0(3) . 1_455
Y2A Se2B Sr2A 0.00(10) 1_455 1_455
Bi5B Se2B Y2C 100.3(3) . 1_455
Sr3A Se2B Y2C 164.6(3) . 1_455
Sr3C Se2B Y2C 96.1(3) . 1_455
Y2A Se2B Y2C 81.7(3) 1_455 1_455
Sr2A Se2B Y2C 81.7(3) 1_455 1_455
Bi5B Se2B Sr2C 100.3(3) . 1_455
Sr3A Se2B Sr2C 164.6(3) . 1_455
Sr3C Se2B Sr2C 96.1(3) . 1_455
Y2A Se2B Sr2C 81.7(3) 1_455 1_455
Sr2A Se2B Sr2C 81.7(3) 1_455 1_455
Y2C Se2B Sr2C 0.0(3) 1_455 1_455
Bi5C Se2C Y3A 95.2(3) . 1_554
Bi5C Se2C Sr3A 95.2(3) . 1_554
Y3A Se2C Sr3A 0.00(11) 1_554 1_554
Bi5C Se2C Sr3B 95.7(3) . .
Y3A Se2C Sr3B 84.4(3) 1_554 .
Sr3A Se2C Sr3B 84.4(3) 1_554 .
Bi5C Se2C Sr2A 99.2(2) . 1_454
Y3A Se2C Sr2A 94.3(3) 1_554 1_454
Sr3A Se2C Sr2A 94.3(3) 1_554 1_454
Sr3B Se2C Sr2A 165.1(3) . 1_454
Bi5C Se2C Y2A 99.2(2) . 1_454
Y3A Se2C Y2A 94.3(3) 1_554 1_454
Sr3A Se2C Y2A 94.3(3) 1_554 1_454
Sr3B Se2C Y2A 165.1(3) . 1_454
Sr2A Se2C Y2A 0.0(3) 1_454 1_454
Bi5C Se2C Sr2B 99.7(3) . 1_455
Y3A Se2C Sr2B 165.1(3) 1_554 1_455
Sr3A Se2C Sr2B 165.1(3) 1_554 1_455
Sr3B Se2C Sr2B 95.4(3) . 1_455
Sr2A Se2C Sr2B 82.0(3) 1_454 1_455
Y2A Se2C Sr2B 82.0(3) 1_454 1_455
Bi5C Se2C Y2B 99.7(3) . 1_455
Y3A Se2C Y2B 165.1(3) 1_554 1_455
Sr3A Se2C Y2B 165.1(3) 1_554 1_455
Sr3B Se2C Y2B 95.4(3) . 1_455
Sr2A Se2C Y2B 82.0(3) 1_454 1_455
Y2A Se2C Y2B 82.0(3) 1_454 1_455
Sr2B Se2C Y2B 0.0(3) 1_455 1_455
Bi4B Se3A Y1B 100.3(3) . 3
Bi4B Se3A Sr1B 100.3(3) . 3
Y1B Se3A Sr1B 0.0(3) 3 3
Bi4B Se3A Y1C 100.2(3) . 4_655
Y1B Se3A Y1C 85.56(11) 3 4_655
Sr1B Se3A Y1C 85.56(11) 3 4_655
Bi4B Se3A Sr1C 100.2(3) . 4_655
Y1B Se3A Sr1C 85.56(11) 3 4_655
Sr1B Se3A Sr1C 85.56(11) 3 4_655
Y1C Se3A Sr1C 0.0(4) 4_655 4_655
Bi4B Se3A Y3B 90.7(2) . 3
Y1B Se3A Y3B 94.2(4) 3 3
Sr1B Se3A Y3B 94.2(4) 3 3
Y1C Se3A Y3B 168.9(2) 4_655 3
Sr1C Se3A Y3B 168.9(2) 4_655 3
Bi4B Se3A Sr3B 90.7(2) . 3
Y1B Se3A Sr3B 94.2(4) 3 3
Sr1B Se3A Sr3B 94.2(4) 3 3
Y1C Se3A Sr3B 168.9(2) 4_655 3
Sr1C Se3A Sr3B 168.9(2) 4_655 3
Y3B Se3A Sr3B 0.0(4) 3 3
Bi4B Se3A Y3C 90.0(3) . 3
Y1B Se3A Y3C 169.4(2) 3 3
Sr1B Se3A Y3C 169.4(2) 3 3
Y1C Se3A Y3C 95.0(4) 4_655 3
Sr1C Se3A Y3C 95.0(4) 4_655 3
Y3B Se3A Y3C 83.25(8) 3 3
Sr3B Se3A Y3C 83.25(8) 3 3
Bi4B Se3A Sr3C 90.0(3) . 3
Y1B Se3A Sr3C 169.4(2) 3 3
Sr1B Se3A Sr3C 169.4(2) 3 3
Y1C Se3A Sr3C 95.0(4) 4_655 3
Sr1C Se3A Sr3C 95.0(4) 4_655 3
Y3B Se3A Sr3C 83.25(8) 3 3
Sr3B Se3A Sr3C 83.25(8) 3 3
Y3C Se3A Sr3C 0.0(4) 3 3
Ge4A Se3B Y1A 101.4(4) . 4_655
Ge4A Se3B Sr1A 101.4(4) . 4_655
Y1A Se3B Sr1A 0.0(3) 4_655 4_655
Ge4A Se3B Y1C 102.3(4) . 4_655
Y1A Se3B Y1C 84.0(3) 4_655 4_655
Sr1A Se3B Y1C 84.0(3) 4_655 4_655
Ge4A Se3B Sr1C 102.3(4) . 4_655
Y1A Se3B Sr1C 84.0(3) 4_655 4_655
Sr1A Se3B Sr1C 84.0(3) 4_655 4_655
Y1C Se3B Sr1C 0.0(4) 4_655 4_655
Ge4A Se3B Y3A 87.6(3) . 3
Y1A Se3B Y3A 99.3(3) 4_655 3
Sr1A Se3B Y3A 99.3(3) 4_655 3
Y1C Se3B Y3A 168.8(4) 4_655 3
Sr1C Se3B Y3A 168.8(4) 4_655 3
Ge4A Se3B Sr3A 87.6(3) . 3
Y1A Se3B Sr3A 99.3(3) 4_655 3
Sr1A Se3B Sr3A 99.3(3) 4_655 3
Y1C Se3B Sr3A 168.8(4) 4_655 3
Sr1C Se3B Sr3A 168.8(4) 4_655 3
Y3A Se3B Sr3A 0.00(10) 3 3
Ge4A Se3B Y3C 88.6(4) . 3
Y1A Se3B Y3C 170.0(4) 4_655 3
Sr1A Se3B Y3C 170.0(4) 4_655 3
Y1C Se3B Y3C 94.2(3) 4_655 3
Sr1C Se3B Y3C 94.2(3) 4_655 3
Y3A Se3B Y3C 80.8(3) 3 3
Sr3A Se3B Y3C 80.8(3) 3 3
Ge4A Se3B Sr3C 88.6(4) . 3
Y1A Se3B Sr3C 170.0(4) 4_655 3
Sr1A Se3B Sr3C 170.0(4) 4_655 3
Y1C Se3B Sr3C 94.2(3) 4_655 3
Sr1C Se3B Sr3C 94.2(3) 4_655 3
Y3A Se3B Sr3C 80.8(3) 3 3
Sr3A Se3B Sr3C 80.8(3) 3 3
Y3C Se3B Sr3C 0.0(4) 3 3
Ge4C Se3C Y1B 100.6(4) . 3_556
Ge4C Se3C Sr1B 100.6(4) . 3_556
Y1B Se3C Sr1B 0.0(3) 3_556 3_556
Ge4C Se3C Sr1A 101.9(4) . 4_655
Y1B Se3C Sr1A 84.7(3) 3_556 4_655
Sr1B Se3C Sr1A 84.7(3) 3_556 4_655
Ge4C Se3C Y1A 101.9(4) . 4_655
Y1B Se3C Y1A 84.7(3) 3_556 4_655
Sr1B Se3C Y1A 84.7(3) 3_556 4_655
Sr1A Se3C Y1A 0.0(3) 4_655 4_655
Ge4C Se3C Y3A 88.8(3) . 3
Y1B Se3C Y3A 168.9(3) 3_556 3
Sr1B Se3C Y3A 168.9(3) 3_556 3
Sr1A Se3C Y3A 99.2(3) 4_655 3
Y1A Se3C Y3A 99.2(3) 4_655 3
Ge4C Se3C Sr3A 88.8(3) . 3
Y1B Se3C Sr3A 168.9(3) 3_556 3
Sr1B Se3C Sr3A 168.9(3) 3_556 3
Sr1A Se3C Sr3A 99.2(3) 4_655 3
Y1A Se3C Sr3A 99.2(3) 4_655 3
Y3A Se3C Sr3A 0.00(11) 3 3
Ge4C Se3C Y3B 88.4(4) . 3_556
Y1B Se3C Y3B 92.9(3) 3_556 3_556
Sr1B Se3C Y3B 92.9(3) 3_556 3_556
Sr1A Se3C Y3B 169.7(3) 4_655 3_556
Y1A Se3C Y3B 169.7(3) 4_655 3_556
Y3A Se3C Y3B 81.5(3) 3 3_556
Sr3A Se3C Y3B 81.5(3) 3 3_556
Ge4C Se3C Sr3B 88.4(4) . 3_556
Y1B Se3C Sr3B 92.9(3) 3_556 3_556
Sr1B Se3C Sr3B 92.9(3) 3_556 3_556
Sr1A Se3C Sr3B 169.7(3) 4_655 3_556
Y1A Se3C Sr3B 169.7(3) 4_655 3_556
Y3A Se3C Sr3B 81.5(3) 3 3_556
Sr3A Se3C Sr3B 81.5(3) 3 3_556
Y3B Se3C Sr3B 0.0(3) 3_556 3_556
Bi5C Se4A Bi5A 97.5(3) . .
Bi5C Se4A Bi6B 93.5(3) . .
Bi5A Se4A Bi6B 94.3(3) . .
Bi5C Se4A Sr3B 94.2(3) . .
Bi5A Se4A Sr3B 93.6(3) . .
Bi6B Se4A Sr3B 168.2(4) . .
Bi5C Se4A Sr1B 131.0(3) . .
Bi5A Se4A Sr1B 131.3(3) . .
Bi6B Se4A Sr1B 80.5(2) . .
Sr3B Se4A Sr1B 87.8(3) . .
Bi5A Se4B Bi5B 97.9(3) . .
Bi5A Se4B Bi6C 94.3(3) . 2_655
Bi5B Se4B Bi6C 93.3(3) . 2_655
Bi5A Se4B Sr3C 94.3(3) . .
Bi5B Se4B Sr3C 94.2(3) . .
Bi6C Se4B Sr3C 167.7(4) 2_655 .
Bi5A Se4B Sr1C 131.2(3) . 2_655
Bi5B Se4B Sr1C 130.5(3) . 2_655
Bi6C Se4B Sr1C 78.8(2) 2_655 2_655
Sr3C Se4B Sr1C 88.9(3) . 2_655
Bi5B Se4C Bi5C 99.40(9) . 1_556
Bi5B Se4C Bi6A 95.9(2) . 2_655
Bi5C Se4C Bi6A 95.5(2) 1_556 2_655
Bi5B Se4C Sr3A 92.4(3) . .
Bi5C Se4C Sr3A 92.1(3) 1_556 .
Bi6A Se4C Sr3A 167.67(11) 2_655 .
Bi5B Se4C Sr1A 130.7(4) . 2_655
Bi5C Se4C Sr1A 129.7(4) 1_556 2_655
Bi6A Se4C Sr1A 77.28(8) 2_655 2_655
Sr3A Se4C Sr1A 90.40(9) . 2_655
Bi4B Se5A Sr2C 95.5(3) . .
Bi4B Se5A Sr2B 95.9(3) . .
Sr2C Se5A Sr2B 83.81(9) . .
Bi4B Se5A Y3B 89.3(2) . 3
Sr2C Se5A Y3B 175.1(2) . 3
Sr2B Se5A Y3B 97.1(4) . 3
Bi4B Se5A Sr3B 89.3(2) . 3
Sr2C Se5A Sr3B 175.1(2) . 3
Sr2B Se5A Sr3B 97.1(4) . 3
Y3B Se5A Sr3B 0.0(4) 3 3
Bi4B Se5A Y3C 88.6(2) . 3
Sr2C Se5A Y3C 96.3(4) . 3
Sr2B Se5A Y3C 175.5(2) . 3
Y3B Se5A Y3C 82.37(8) 3 3
Sr3B Se5A Y3C 82.37(8) 3 3
Bi4B Se5A Sr3C 88.6(2) . 3
Sr2C Se5A Sr3C 96.3(4) . 3
Sr2B Se5A Sr3C 175.5(2) . 3
Y3B Se5A Sr3C 82.37(8) 3 3
Sr3B Se5A Sr3C 82.37(8) 3 3
Y3C Se5A Sr3C 0.0(4) 3 3
Ge4A Se5B Sr2A 107.0(4) . .
Ge4A Se5B Sr2C 110.5(4) . .
Sr2A Se5B Sr2C 82.2(3) . .
Ge4A Se5B Y3C 87.2(3) . 3
Sr2A Se5B Y3C 165.6(3) . 3
Sr2C Se5B Y3C 94.9(3) . 3
Ge4A Se5B Sr3C 87.2(3) . 3
Sr2A Se5B Sr3C 165.6(3) . 3
Sr2C Se5B Sr3C 94.9(3) . 3
Y3C Se5B Sr3C 0.0(4) 3 3
Ge4A Se5B Sr3A 84.0(3) . 3
Sr2A Se5B Sr3A 101.0(3) . 3
Sr2C Se5B Sr3A 163.8(4) . 3
Y3C Se5B Sr3A 78.0(3) 3 3
Sr3C Se5B Sr3A 78.0(3) 3 3
Ge4A Se5B Y3A 84.0(3) . 3
Sr2A Se5B Y3A 101.0(3) . 3
Sr2C Se5B Y3A 163.8(4) . 3
Y3C Se5B Y3A 78.0(3) 3 3
Sr3C Se5B Y3A 78.0(3) 3 3
Sr3A Se5B Y3A 0.00(10) 3 3
Ge4C Se5C Sr2A 107.7(4) . .
Ge4C Se5C Y2B 109.8(4) . 1_556
Sr2A Se5C Y2B 81.6(3) . 1_556
Ge4C Se5C Sr2B 109.8(4) . 1_556
Sr2A Se5C Sr2B 81.6(3) . 1_556
Y2B Se5C Sr2B 0.0(2) 1_556 1_556
Ge4C Se5C Y3B 87.5(3) . 3_556
Sr2A Se5C Y3B 164.7(3) . 3_556
Y2B Se5C Y3B 94.8(3) 1_556 3_556
Sr2B Se5C Y3B 94.8(3) 1_556 3_556
Ge4C Se5C Sr3B 87.5(3) . 3_556
Sr2A Se5C Sr3B 164.7(3) . 3_556
Y2B Se5C Sr3B 94.8(3) 1_556 3_556
Sr2B Se5C Sr3B 94.8(3) 1_556 3_556
Y3B Se5C Sr3B 0.0(3) 3_556 3_556
Ge4C Se5C Sr3A 85.3(3) . 3
Sr2A Se5C Sr3A 100.7(3) . 3
Y2B Se5C Sr3A 163.5(3) 1_556 3
Sr2B Se5C Sr3A 163.5(3) 1_556 3
Y3B Se5C Sr3A 78.6(3) 3_556 3
Sr3B Se5C Sr3A 78.6(3) 3_556 3
Ge4C Se5C Y3A 85.3(3) . 3
Sr2A Se5C Y3A 100.7(3) . 3
Y2B Se5C Y3A 163.5(3) 1_556 3
Sr2B Se5C Y3A 163.5(3) 1_556 3
Y3B Se5C Y3A 78.6(3) 3_556 3
Sr3B Se5C Y3A 78.6(3) 3_556 3
Sr3A Se5C Y3A 0.00(10) 3 3
Bi6A Se6A Bi6C 92.1(3) . .
Bi6A Se6A Bi5C 174.8(4) . 1_655
Bi6C Se6A Bi5C 89.0(2) . 1_655
Bi6A Se6A Bi5A 90.7(2) . 1_655
Bi6C Se6A Bi5A 174.0(4) . 1_655
Bi5C Se6A Bi5A 87.7(3) 1_655 1_655
Bi6A Se6A Sr2B 91.0(3) . .
Bi6C Se6A Sr2B 91.9(3) . .
Bi5C Se6A Sr2B 94.0(3) 1_655 .
Bi5A Se6A Sr2B 93.3(3) 1_655 .
Bi6A Se6B Bi6B 92.1(3) . 2_655
Bi6A Se6B Bi5A 90.9(3) . 1_655
Bi6B Se6B Bi5A 174.0(3) 2_655 1_655
Bi6A Se6B Bi5B 175.0(3) . 1_655
Bi6B Se6B Bi5B 88.6(2) 2_655 1_655
Bi5A Se6B Bi5B 87.9(3) 1_655 1_655
Bi6A Se6B Sr2C 91.1(3) . .
Bi6B Se6B Sr2C 91.2(3) 2_655 .
Bi5A Se6B Sr2C 93.8(3) 1_655 .
Bi5B Se6B Sr2C 93.8(3) 1_655 .
Bi6C Se6C Bi6B 90.41(7) 1_556 2_655
Bi6C Se6C Bi5C 90.0(3) 1_556 1_656
Bi6B Se6C Bi5C 178.28(16) 2_655 1_656
Bi6C Se6C Bi5B 178.24(14) 1_556 1_655
Bi6B Se6C Bi5B 89.8(3) 2_655 1_655
Bi5C Se6C Bi5B 89.68(7) 1_656 1_655
Bi6C Se6C Sr2A 90.1(2) 1_556 .
Bi6B Se6C Sr2A 89.9(2) 2_655 .
Bi5C Se6C Sr2A 91.8(2) 1_656 .
Bi5B Se6C Sr2A 91.7(2) 1_655 .
Bi6C Se7A Bi6B 94.45(9) 2_655 .
Bi6C Se7A Sr1A 91.2(2) 2_655 .
Bi6B Se7A Sr1A 90.4(2) . .
Bi6C Se7A Y1C 87.3(3) 2_655 2_655
Bi6B Se7A Y1C 150.9(2) . 2_655
Sr1A Se7A Y1C 118.6(3) . 2_655
Bi6C Se7A Sr1C 87.3(3) 2_655 2_655
Bi6B Se7A Sr1C 150.9(2) . 2_655
Sr1A Se7A Sr1C 118.6(3) . 2_655
Y1C Se7A Sr1C 0.0(3) 2_655 2_655
Bi6C Se7A Sr1B 149.72(19) 2_655 .
Bi6B Se7A Sr1B 85.9(3) . .
Sr1A Se7A Sr1B 119.1(3) . .
Y1C Se7A Sr1B 78.50(9) 2_655 .
Sr1C Se7A Sr1B 78.50(9) 2_655 .
Bi6C Se7B Bi6A 94.1(3) . .
Bi6C Se7B Sr1B 93.1(3) . .
Bi6A Se7B Sr1B 88.4(3) . .
Bi6C Se7B Sr1C 88.2(3) . .
Bi6A Se7B Sr1C 148.6(4) . .
Sr1B Se7B Sr1C 122.8(4) . .
Bi6C Se7B Sr1A 150.4(4) . .
Bi6A Se7B Sr1A 83.1(2) . .
Sr1B Se7B Sr1A 116.1(3) . .
Sr1C Se7B Sr1A 79.7(3) . .
Bi6A Se7C Bi6B 94.8(3) 2_654 .
Bi6A Se7C Sr1C 90.2(3) 2_654 .
Bi6B Se7C Sr1C 91.1(3) . .
Bi6A Se7C Y1A 86.5(3) 2_654 2_654
Bi6B Se7C Y1A 150.2(4) . 2_654
Sr1C Se7C Y1A 118.7(3) . 2_654
Bi6A Se7C Sr1A 86.5(3) 2_654 2_654
Bi6B Se7C Sr1A 150.2(4) . 2_654
Sr1C Se7C Sr1A 118.7(3) . 2_654
Y1A Se7C Sr1A 0.00(10) 2_654 2_654
Bi6A Se7C Sr1B 148.5(4) 2_654 .
Bi6B Se7C Sr1B 84.8(3) . .
Sr1C Se7C Sr1B 121.3(4) . .
Y1A Se7C Sr1B 79.0(3) 2_654 .
Sr1A Se7C Sr1B 79.0(3) 2_654 .
Ge4C Se8A Ge4A 108.90(13) 1_455 1_455
Ge4C Se8A Sr3A 112.3(4) 1_455 .
Ge4A Se8A Sr3A 110.3(4) 1_455 .
Ge4C Se8B Bi4B 115.4(4) 1_454 1_455
Ge4C Se8B Sr3B 118.8(4) 1_454 .
Bi4B Se8B Sr3B 92.8(3) 1_455 .
Ge4C Se8B Sr1B 84.1(3) 1_454 3_455
Bi4B Se8B Sr1B 81.8(2) 1_455 3_455
Sr3B Se8B Sr1B 156.2(3) . 3_455
Ge4A Se8C Bi4B 114.7(4) 1_455 1_455
Ge4A Se8C Sr3C 120.5(4) 1_455 .
Bi4B Se8C Sr3C 91.4(3) 1_455 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sr1A Se7A 3.104(4) .
Sr1A Se1C 3.140(11) 2_655
Sr1A Se1B 3.147(11) .
Sr1A Se3B 3.189(11) 4_644
Sr1A Se3C 3.201(11) 4_644
Sr1A Se7C 3.284(11) 2_655
Sr1A Se7B 3.373(11) .
Sr1A Se4C 3.682(4) 2_654
Sr1A Sr1C 4.280(13) .
Sr1A Sr1B 4.282(12) 2_655
Sr1A Y1B 4.282(12) 2_655
Sr1B Se3A 3.127(11) 3_455
Sr1B Se3C 3.155(11) 3_454
Sr1B Se1A 3.161(11) .
Sr1B Se1C 3.202(12) .
Sr1B Se7B 3.269(12) .
Sr1B Se7A 3.434(10) .
Sr1B Se7C 3.445(12) .
Sr1B Se4A 3.580(12) .
Sr1B Se8B 3.811(12) 3
Sr1B Sr1A 4.282(12) 2_654
Sr1B Y1A 4.282(12) 2_654
Sr1B Sr1C 4.297(4) 2_655
Sr1C Se1A 3.155(12) 2_654
Sr1C Se7C 3.177(14) .
Sr1C Se1B 3.180(12) .
Sr1C Se3A 3.198(12) 4_644
Sr1C Se3B 3.211(13) 4_644
Sr1C Se7B 3.304(13) .
Sr1C Se7A 3.356(12) 2_654
Sr1C Se4B 3.637(12) 2_654
Sr1C Y1B 4.297(4) 2_654
Sr1C Sr1B 4.297(4) 2_654
Sr2A Se1C 3.189(12) 1_556
Sr2A Se1B 3.191(12) 2_655
Sr2A Se2C 3.230(11) 1_656
Sr2A Se2B 3.233(12) 1_655
Sr2A Se5B 3.238(11) .
Sr2A Se5C 3.251(11) .
Sr2A Se6C 3.266(3) .
Sr2A Sr2C 4.264(13) .
Sr2A Sr2B 4.276(12) 1_556
Sr2A Y2B 4.276(12) 1_556
Sr2A Sr3A 4.680(3) 1_655
Sr2B Se1A 3.192(12) .
Sr2B Se1C 3.222(13) .
Sr2B Se6A 3.224(13) .
Sr2B Se5A 3.231(11) .
Sr2B Se2A 3.264(11) 1_655
Sr2B Se2C 3.286(12) 1_655
Sr2B Se5C 3.292(12) 1_554
Sr2B Y2A 4.276(12) 1_554
Sr2B Sr2A 4.276(12) 1_554
Sr2B Sr2C 4.311(4) .
Sr2C Se1B 3.199(12) 2_655
Sr2C Se1A 3.223(12) .
Sr2C Se5A 3.224(12) .
Sr2C Se5B 3.249(12) .
Sr2C Se6B 3.253(11) .
Sr2C Se2B 3.283(12) 1_655
Sr2C Se2A 3.313(11) 1_655
Sr2C Sr1C 4.646(12) 2_655
Sr3A Se2B 3.145(12) .
Sr3A Se2C 3.153(11) 1_556
Sr3A Se4C 3.183(4) .
Sr3A Se3C 3.213(11) 3_455
Sr3A Se3B 3.220(11) 3_455
Sr3A Se8A 3.288(4) .
Sr3A Se5B 3.366(11) 3_455
Sr3A Se5C 3.367(11) 3_455
Sr3A Sr3C 4.231(13) .
Sr3A Y3B 4.264(12) 1_556
Sr3A Sr3B 4.264(12) 1_556
Sr3B Se4A 3.173(12) .
Sr3B Se2C 3.196(12) .
Sr3B Se2A 3.196(11) .
Sr3B Se8B 3.247(12) .
Sr3B Se3A 3.274(12) 3_455
Sr3B Se5A 3.304(12) 3_455
Sr3B Se3C 3.318(12) 3_454
Sr3B Se5C 3.362(12) 3_454
Sr3B Bi4B 4.245(9) 3_455
Sr3B Sr3A 4.264(12) 1_554
Sr3B Y3A 4.264(12) 1_554
Sr3C Se4B 3.166(12) .
Sr3C Se2B 3.194(12) .
Sr3C Se2A 3.242(11) .
Sr3C Se8C 3.260(12) .
Sr3C Se3A 3.282(12) 3_455
Sr3C Se5A 3.310(12) 3_455
Sr3C Se3B 3.311(13) 3_455
Sr3C Se5B 3.358(12) 3_455
Sr3C Bi4B 4.226(9) 3_455
Ge4A Se8C 2.312(12) 1_655
Ge4A Se3B 2.354(13) .
Ge4A Se5B 2.367(13) .
Ge4A Se8A 2.455(12) 1_655
Bi4B Se3A 2.661(3) .
Bi4B Se5A 2.709(3) .
Bi4B Se8B 2.913(9) 1_655
Bi4B Se8C 2.973(9) 1_655
Bi4B Sr3C 4.226(9) 3
Bi4B Sr3B 4.245(9) 3
Ge4C Se5C 2.343(12) .
Ge4C Se3C 2.350(12) .
Ge4C Se8B 2.352(11) 1_656
Ge4C Se8A 2.411(13) 1_655
Bi5A Se2A 2.779(3) .
Bi5A Se4B 2.822(9) .
Bi5A Se4A 2.832(9) .
Bi5A Se6B 3.059(9) 1_455
Bi5A Se6A 3.073(9) 1_455
Bi5B Se2B 2.725(9) .
Bi5B Se4C 2.820(10) .
Bi5B Se4B 2.834(9) .
Bi5B Se6C 3.071(9) 1_455
Bi5B Se6B 3.083(9) 1_455
Bi5C Se2C 2.726(9) .
Bi5C Se4A 2.831(9) .
Bi5C Se4C 2.854(10) 1_554
Bi5C Se6C 3.065(9) 1_454
Bi5C Se6A 3.073(10) 1_455
Bi6A Se1A 2.770(3) .
Bi6A Se7C 2.909(11) 2_655
Bi6A Se6A 2.964(10) .
Bi6A Se6B 2.966(10) .
Bi6A Se7B 3.028(11) .
Bi6A Se4C 3.087(3) 2_654
Bi6B Se1B 2.759(9) .
Bi6B Se7A 2.895(9) .
Bi6B Se7C 2.957(9) .
Bi6B Se6C 2.978(9) 2_654
Bi6B Se6B 3.032(9) 2_654
Bi6B Se4A 3.101(9) .
Bi6C Se1C 2.761(9) .
Bi6C Se7A 2.855(8) 2_654
Bi6C Se7B 2.858(9) .
Bi6C Se6C 2.971(9) 1_554
Bi6C Se6A 3.019(9) .
Bi6C Se4B 3.106(9) 2_654
Se1A Y1C 3.155(12) 2_655
Se1A Sr1C 3.155(12) 2_655
Se1B Y2A 3.191(12) 2_654
Se1B Sr2A 3.191(12) 2_654
Se1B Y2C 3.199(12) 2_654
Se1B Sr2C 3.199(12) 2_654
Se1C Y1A 3.140(11) 2_654
Se1C Sr1A 3.140(11) 2_654
Se1C Y2A 3.189(12) 1_554
Se1C Sr2A 3.189(12) 1_554
Se2A Y2B 3.264(11) 1_455
Se2A Sr2B 3.264(11) 1_455
Se2A Y2C 3.313(11) 1_455
Se2A Sr2C 3.313(11) 1_455
Se2B Y2A 3.233(12) 1_455
Se2B Sr2A 3.233(12) 1_455
Se2B Y2C 3.283(12) 1_455
Se2B Sr2C 3.283(12) 1_455
Se2C Y3A 3.153(11) 1_554
Se2C Sr3A 3.153(11) 1_554
Se2C Sr2A 3.230(11) 1_454
Se2C Y2A 3.230(11) 1_454
Se2C Sr2B 3.286(12) 1_455
Se2C Y2B 3.286(12) 1_455
Se3A Y1B 3.127(11) 3
Se3A Sr1B 3.127(11) 3
Se3A Y1C 3.198(12) 4_655
Se3A Sr1C 3.198(12) 4_655
Se3A Y3B 3.274(12) 3
Se3A Sr3B 3.274(12) 3
Se3A Y3C 3.282(12) 3
Se3A Sr3C 3.282(12) 3
Se3B Y1A 3.189(11) 4_655
Se3B Sr1A 3.189(11) 4_655
Se3B Y1C 3.211(13) 4_655
Se3B Sr1C 3.211(13) 4_655
Se3B Y3A 3.220(11) 3
Se3B Sr3A 3.220(11) 3
Se3B Y3C 3.311(13) 3
Se3B Sr3C 3.311(13) 3
Se3C Y1B 3.155(11) 3_556
Se3C Sr1B 3.155(11) 3_556
Se3C Sr1A 3.201(11) 4_655
Se3C Y1A 3.201(11) 4_655
Se3C Y3A 3.213(11) 3
Se3C Sr3A 3.213(11) 3
Se3C Y3B 3.318(12) 3_556
Se3C Sr3B 3.318(12) 3_556
Se4B Bi6C 3.106(9) 2_655
Se4B Sr1C 3.637(12) 2_655
Se4C Bi5C 2.854(10) 1_556
Se4C Bi6A 3.087(3) 2_655
Se4C Sr1A 3.682(4) 2_655
Se5A Y3B 3.304(12) 3
Se5A Sr3B 3.304(12) 3
Se5A Y3C 3.310(12) 3
Se5A Sr3C 3.310(12) 3
Se5B Y3C 3.358(12) 3
Se5B Sr3C 3.358(12) 3
Se5B Sr3A 3.366(11) 3
Se5B Y3A 3.366(11) 3
Se5C Y2B 3.292(12) 1_556
Se5C Sr2B 3.292(12) 1_556
Se5C Y3B 3.362(12) 3_556
Se5C Sr3B 3.362(12) 3_556
Se5C Sr3A 3.367(11) 3
Se5C Y3A 3.367(11) 3
Se6A Bi5C 3.073(10) 1_655
Se6A Bi5A 3.073(9) 1_655
Se6B Bi6B 3.032(9) 2_655
Se6B Bi5A 3.059(9) 1_655
Se6B Bi5B 3.083(9) 1_655
Se6C Bi6C 2.971(9) 1_556
Se6C Bi6B 2.978(9) 2_655
Se6C Bi5C 3.065(9) 1_656
Se6C Bi5B 3.071(9) 1_655
Se7A Bi6C 2.855(8) 2_655
Se7A Y1C 3.356(12) 2_655
Se7A Sr1C 3.356(12) 2_655
Se7C Bi6A 2.909(11) 2_654
Se7C Y1A 3.284(11) 2_654
Se7C Sr1A 3.284(11) 2_654
Se8A Ge4C 2.411(13) 1_455
Se8A Ge4A 2.455(12) 1_455
Se8B Ge4C 2.352(11) 1_454
Se8B Bi4B 2.913(9) 1_455
Se8B Sr1B 3.811(12) 3_455
Se8C Ge4A 2.312(12) 1_455
Se8C Bi4B 2.973(9) 1_455
